N A N O E X P R E S S
Synthesis of ZnO/Si Hierarchical Nanowire
Arrays for Photocatalyst Application
, Xiaolan Yan1†
, Chunhua Lin2
, Shengli Huang1,2,3,4*
, Z. Ryan Tian2
, Bing He1
, Qianqian Yang1
, Xu He1
, Jing Li1
, Jiayuan Wang1
, Huahan Zhan1
, Shuping Li1
and Junyong Kang1
ZnO/Si nanowire arrays with hierarchical architecture were synthesized by solution method with ZnO seed layer grown by atomic layer deposition and magnetron sputtering, respectively. The photocatalytic activity of the as-grown tree-like arrays was evaluated by the degradation of methylene blue under ultraviolet light at ambient temperature. The comparison of morphology, crystal structure, optical properties, and photocatalysis efficiency of the two samples in different seeding processes was conducted. It was found that the ZnO/Si nanowire arrays presented a larger surface area with better crystalline and more uniform ZnO branches on the whole sidewall of Si backbones for the seed layer by atomic layer deposition, which gained a strong light absorption as high as 98% in the ultraviolet and visible range. The samples were proven to have a potential use in photocatalyst, but suffered from photodissolution and memory effect. The mechanism of the photocatalysis was analyzed, and the stability and recycling ability were also evaluated and enhanced.
Keywords:Photocatalytic activity, Nanowire arrays, Hierarchical architecture, Semiconductor
Along with social development, the environmental pollu-tion is becoming more and more critical. Finding a high efficient and cost-effective catalyst is one of the best ways to remove the pollutants such as organic dyes and toxic chemicals. Semiconductor photocatalysts are the key materials to complete mineralization of a wide range of dyes and organic compounds, as they offer tunable and enhanced photoresponse in ultraviolet (UV) and vis-ible region and efficient electron-hole separation to cre-ate active radicals for photocatalysis . Among the semiconductor materials studied, hybrid nanowires with different materials have been of great interest due to the potential superior efficiency coming from the unique geometry and properties, unlimited combination, and ef-fective integration at nanoscale to implement design and
material integrity . In this regard, branched tree-like nanowire arrays may be the most favorite choice because they provide omnidirectional branches for effective pho-ton absorption, enlarge surface area to react with the pollutants, maximize junction interface area for electron-hole separation, and enhance surface curvature for a high reaction kinetics [3–5].
Semiconductor materials that are currently applied in the building blocks of functional hybrid nanowire arrays includes Si [6–8], Ge , III–V [10–12], IV–VI [13, 14], II–VI [15, 16] and metal oxides (ZnO [2, 17–21], TiO2
, In2O3, and Fe2O3). Among them, Si is the
most fundamental material in current photovoltaic mar-ket and has demonstrated broad application as solar cell, sensor, and catalyst. However, the potential corrosion and high valence band maximum energy make it unsuit-able alone in these fields. Another semiconductor mater-ial, ZnO, may be a good candidate to remedy these problems for its large bandgap (3.37 eV), large exciton binding energy (60 meV), and stable physical and chem-ical properties. Moreover, it is easily obtained in different types of nanostructures. Previously research on the ZnO/Si nanowire arrays found a very high photovoltaic current density and efficiency [17–20]. Study of the * Correspondence:firstname.lastname@example.org
1Fujian Provincial Key Laboratory of Semiconductors and Applications,
Collaborative Innovation Center for Optoelectronic Semiconductors and Efficient Devices, Department of Physics, Xiamen University, Xiamen 361005, China
2Department of Chemistry and Biochemistry, University of Arkansas,
Fayetteville, AR 72701, USA
Full list of author information is available at the end of the article
system currently concentrates on the photovoltaics , dye-sensitized solar cells , photoelectrochemical electrodes for water splitting [18, 20], and sensors , but literature about photocatalytic activity is rarely re-ported . In this research, the arrays were used as a catalyst to degrade methyl red and exhibited a good photocatalytic capability. However, the arrays were grown by both chemical etching and chemical vapor de-position. Photolithography was also applied in order to fabricate patterned Si arrays in a controlled geometry and density. All these costed much time and needed so-phisticated equipments. In our experiment, except the seed layer, we used solution method to grow the hybrid nanowire arrays, owning the advantages of low synthetic temperature, simple equipment, and time saving.
In the fabrication of hybrid nanowire arrays, the seed layer is a vital factor, because it decides the position, diameter, orientation, and density of the nanowire arrays. In previous research, the seed layer of the branched ZnO nanowires was respectively deposited by magnetron sputtering (MS) , electrospinning , spin coating , dip coating , as well as atomic layer deposition (ALD) . All these reports are chiefly concerning on the final function of the ZnO/Si nanowire arrays. The optimization of the seed layer has yet to be resolved.
Therefore, in this article, two different seeding methods were used to figure out how it influence the growth of branched ZnO nanowires as well as the properties and function of tree-like ZnO/Si nanowire arrays. One seeding method was ALD, while the other one was MS. The photocatalytic activity of the as-grown tree-like ZnO/Si nanowire arrays was evaluated by the degradation of a typ-ical organic dye methylene blue (MB) under UV light ir-radiation. The comparison of morphology, crystal structure, optical properties, and photocatalysis efficiency of the two samples was conducted. Moreover, the mech-anism of the photocatalysis was analyzed, and the stability and recycling ability were also evaluated.
The fabrication process of ZnO/Si nanowire arrays in-cludes substrate cleaning, wet chemical etching for Si backbones, ZnO seed layer deposition, and ZnO branches growth. First, P-type boron doped (100) Si wa-fers with resistivity of 1–10 Ω cm and thickness of 450 μm were used as substrates for the synthesis of the hybrid structure. The substrates were cut in a size of 10 × 15 mm2and sequentially cleaned by ultrasonication in absolute toluene, acetone, ethanol, and piranha solu-tion (H2SO4and H2O2in a volume ratio of 3:1) at 80 °C
for 2 h, each of which was followed by ultrasonication in de-ionized water.
Second, after the substrates were dried with N2 flow,
they were immersed in aqueous solution of 4 M HF and 0.02 M AgNO3in a Teflon vessel for a galvanic
displace-ment reaction at 50 °C for 30 min. The post-etched sub-strates were transferred to the solution of HCl/HNO3/
H2O in a volume ratio of 1:1:1 overnight to remove the
reduced Ag nanoparticles during the chemical etching. The substrates were then thoroughly rinsed with de-ionized water and dried in air.
Third, the substrates were divided into two equal groups to grow ZnO seed layer by applying the two different methods. One group, denoted as sample ALD, was depos-ited using TALD-100A ALD system (Keming Co. Ltd., China), while the other one, denoted as sample MS, was grown using JC500-3/D MS system (Chaomai Co. Ltd., China). In detail, to make sample ALD, the reactive cham-ber of the ALD system was preheated in nitrogen atmos-phere at 100 °C for 24 h, then the substrates were placed into the chamber. Afterwards, the pressure of the chamber was pumped to 0.15 torr followed by heated to 150 °C. The 167 cycles of Zn(C2H5)2dose for 0.02 s, N2flow for 25 s,
water vapor dose for 0.015 s, and N2flow for 25 s were
re-quired to grow a ZnO seed layer with 30 nm thickness. As for sample MS, the substrates were transferred into a MS chamber in argon carrier gas. The background pressure was evacuated to be 10−4Pa, and the working pressure was set at 1 Pa. The ZnO target was pre-sputtered for 10 min to gain a clean surface, then the seed layer was deposited on the substrates for 3 min at room temperature with sput-tering power of 80 W. The film thickness was character-ized to be about 30 nm by a planar Si substrate.
Fourth, ZnO nanowires were synthesized by hydro-thermal method. A 500-ml aqueous solution of 25 mM Zn(CH3COO)2.2H2O and 25 mM C6H12N4 was filled
into a glass beaker, which was agitated and heated in a magnetic stirring apparatus. After the temperature kept stable at 90 °C, the seeded substrates were soaked verti-cally in the solution for a period of 40 min. The as-grown samples were removed from the solution and rinsed with de-ionized water several times, then they were annealed at 420 °C for 30 min in an oven to obtain ZnO nanowires with better crystallinity.
325 nm. The parameters of PMT voltage, scan speed, and slit width were set at 700 V, 240 nm/min, and 5.0 nm for all the samples. Diffuse reflection spectra and absorption spectra were taken on an Agilent Carry-5000 UV-Vis-NIR spectrophotometer. X-ray photoelectron spectroscopy (XPS) was recorded in a PHI Quantum 2000 with Al Kα X-ray excitation source (hv= 1486.6 eV). All the measure-ments were carried out at room temperature in normal conditions.
The photocatalytic activity of the nanowire arrays was evaluated by the degradation of MB dye under UV light irradiation at ambient temperature. Aqueous suspension of MB (1 × 10−5 M) in a volume of 20 ml was poured into a glass petri dish with a diameter of 85 mm, then a piece of sample was immersed in the solution with the nanowires facing upwards. They were subjected to UV light in an intensity of ~4.5 mW/cm2. The photodegra-dation was performed 1 h per time, and three successive reaction periods on the MB solution with identical concentration were conducted for each sample. The
photocatalytic efficiency was analyzed by measuring ab-sorption spectra of the degraded MB solution.
For the enhancement of photocatalytic activity and re-cycling ability, the surface of sample ALD was coated by a layer of Ag particles and TiO2film. The Ag particles
were reduced by immersing the sample in a suspension of Na3C6H5O7.2H2O and AgNO3in a mole ratio of 20/
2 mM in 100 mL de-ionized water, then irradiated by sun light in an intensity of ~23.5 mW/cm2for an hour . The sample was rinsed several times in de-ionized water and dried in air. Afterwards, a layer of TiO2 film
with 10 nm thickness was deposited on it by ALD. The sample was finally annealed at 400 °C in nitrogen atmos-phere for 3 min in an oven.
Results and Discussion
Morphology and Crystal Structure
Figure 1 shows the SEM images of sample ALD and sample MS after hydrothermal growth. The top view and cross-sectional view of sample ALD (Fig. 1a, c) re-veal that ZnO nanowires uniformly grow along the nor-mal direction on the surface of Si nanowires and even in the bottom between Si nanowires. The length of the[image:3.595.61.538.383.712.2]
ZnO nanowires is 500 nm approximately, while their diameter is in a limited range of 30–50 nm. They own a smooth surface, which suggests good crystallinity and uniform crystal orientation, and is beneficial to the con-duction of the injected electrons and may enhance the photocatalytic performances. However, for sample MS (Fig. 1b, d), the ZnO nanowires only stand on the top part of Si nanowires. There is a clear variation in diam-eter and length of ZnO nanowires in different positions. For the tip area of Si nanowires, the ZnO nanowires are about 1μm in length and 100–200 nm in diameter, exhi-biting a greater magnitude as compared with sample ALD. For the area below the tip end, lots of ZnO nano-wires are also observed with smaller size. All these cause a non-uniformity of distribution, length, and diameter of ZnO branches on the Si backbones. Moreover, the ZnO nanowires are full of potholes that result in a rough sur-face. It is worthwhile to point out that the Si nanowire backbones have the similar structure and dimension for the two kinds of specimens. They are about 16 μm in length and random in diameter due to the nature of metal-assisted electroless etching method . The etched nanowires possess a quite clean and smooth sur-face without any holes or reduced Ag particles, as ob-served in Fig. 1d.
It has been conjectured that the non-uniform distribu-tion of ZnO nanowires on Si backbones is due to the non-uniformity of Si nanowire diameters, large surface curvature of the Si nanowires, and uneven coating of the ZnO seeding layer as well as the damage during the sample preparation [18, 20]. In order to verify this, EDS spectra of sample ALD and sample MS after seeding[image:4.595.57.537.485.713.2]
process were performed at different positions, as shown in Fig. 2. Except the element C that was reduced from the reagents in the hydrothermal growth, only the sig-nals of O, Zn, and Si elements are detected without any reduced Ag or other impurities. This is further corrobo-rated by the following XRD and XPS analysis wherein no Ag peak is observed in the specimens. The variation of elements Si and Zn and Zn/Si ratio of the two sam-ples as calculated from Fig. 2 are depicted in Fig. 3. In the detected region, the Zn atoms of seeded sample ALD give a concentration increasing from the bottom 11.51% through the middle 15.75% to the top 18.41%, while those of seeded sample MS chiefly centralize on the top of Si nanowires and barely come to the bottom. Their concentration is only 0.65% in the bottom and gets 2.08% on the top. The detected concentration of Si atoms is much larger than that of Zn atoms, especially for sample MS. Therefore, the Zn/Si ratio in the identi-cal positions is obviously different for the two speci-mens. It increases from the bottom 0.251 to the top 0.747 for sample ALD, while it rises from 0.00966 to 0.0409 for sample MS, as shown in Fig. 3b. These distri-bution differences can be well attributed to the film de-position methods. The ALD apparatus deposit films layer by layer with high uniformity and conformality, even on high aspect ratio substrates. Though MS appar-atus can deposit films rapidly, it is not good at film growth on substrates with high curvature effect. The dis-tinct morphology difference of the two kinds of samples may induce unlike properties and performances.
Figure 4 shows the XRD patterns of sample ALD and sample MS. The observed peaks are well indexed to
ZnO crystallographic phase with hexagonal wurtzite crystal structure (JCPDS no. 36-1451). There is an additional diffraction peak corresponding to Si(200) in the pattern of sample ALD, which may result from the exposure of Si nanowire backbones or thin thick-ness of ZnO film. No extra peaks relating to any im-purity or Ag particles are observed, which confirms that the as-grown products are pure ZnO/Si hybrid nanostructures. The diffraction peaks of sample MS are sharper than those of sample ALD, revealing big-ger mean size of sample MS crystalline grains on the basis of Debye–Scherrer formula . However, as the peaks intensity of sample MS is weaker than or equal to that of sample ALD, it cannot deduce that sample MS has a better crystallinity than sample ALD from the XRD patterns. In fact, the crystallinity of sample ALD is better than that of sample MS, as obviously seen in SEM images in Fig. 1 and the fol-lowing PL spectra.
Photoluminescence and Optical Reflection
PL spectra of the two samples are displayed in Fig. 5. Three peaks are obviously observed in the spectrum with wavelength positions of 388, 435, and 548 nm. The first peak at 388 nm corresponds to the band edge lumi-nescence of ZnO crystal , which is red-shifted from the bandgap of bulk ZnO (368 nm, 3.37 eV). The reason may be multifold, including the Si component in the hy-brid nanostructure, the growing method with especial reagents, and the existence of oxygen vacancy in ZnO nanowires  and carbon species as established in EDS spectra. The bandgap reduction suggests that the arrays can absorb much light in a far wider wavelength, which is favorable for photocatalytic and photoelectric perfor-mances. The second and third peaks are ascribed to Zn interstitial atoms  and O vacancies . This is an another evidence of better crystallinity of sample ALD compared with sample MS, as the characteristic peak originating from band edge emission is much stronger,
Fig. 3Concentration variation of elements of Si and Zn (a) and Zn/Si ratio (b) of seeded sample ALD and sample MS at different positions in Fig. 2
Fig. 4XRD patterns of sample ALD and sample MS. The ALD curve was shifted upward in contrast to MS curve for comparison[image:5.595.58.518.104.22.168] [image:5.595.305.539.524.694.2] [image:5.595.57.290.528.704.2]
and the extra peaks corresponding to the defects are weaker for the former than those for the latter.
The reflection spectra of the specimens are shown in Fig. 6. They own a low reflectance across the entire UV and visible range. For sample ALD, the reflectance is lower than 3.7% in the measured wavelengths between 250 and 800 nm, Most of it is stable at 2%. As the sub-strate is opaque, this means that all the other light is absorbed by the specimen. Therefore, the light absorp-tion of sample ALD is as high as 98%, which may result from synergistic band structure of the heterogeneous materials, the light trapping effect for the hierarchical architecture, and the smooth transition of refractive index from air (n= 1) through ZnO branches (n= 2.0) to Si backbones (n= 3.5). There is no significant difference between the two curves in UV region. However, for sam-ple MS, the reflectance gives a sharp jump at the wave-lengths between 360 and 400 nm and is 2 to 3 times larger than that of sample ALD in visible region. The optical bandgap estimated from the jump with Tauc model  is about 388 nm, which agrees well with the result of PL spectra in Fig. 5, as both are due to the elec-tron transition from the valence band to the conduction band of ZnO. The stronger absorption of sample ALD than that of sample MS in the visible region may be assigned to larger total surface area and better morph-ology of ZnO nanowires that uniformly grow on the sidewall of Si nanowires, as obviously seen in Fig. 1.
To measure the photocatalytic activity of the two sam-ples, time-dependent photodegradation of MB solution was conducted. When there was no ZnO/Si nanowire arrays in the solution, the MB dye was stable and no ob-vious degradation was observed under irradiation of the UV light, suggesting that the photoinduced self-sensitized photodegradation of MB was negligible.
Figure 7 shows the absorption spectra of MB aqueous solutions as catalyzed by sample ALD and sample MS. The peak intensity of the post-degradation MB solution is lower than that of original solution, suggesting photo-catalytic activity of the two specimens. However, the photocatalytic efficiency is decreased with an extended period. The relationship between the photocatalytic effi-ciency and the time period is calculated. For the MB so-lution, the absorption intensity at the peak position of ~665 nm can be characterized,
T ¼76179:87Cþ0:01155; ð1Þ
where T is the absorbance and C is the concentration. The efficiency of each degradation is obtained by the fol-lowing formula,
E¼ð1−C=C0Þ 100%; ð2Þ
whereEis the photocatalytic efficiency,Cis the concen-tration of post-degradation MB solution, and C0 is the concentration of an original MB solution. The calculated efficiencies are presented in Table1. In the first catalysis cycle, sample ALD demonstrates an efficiency of 15.26%. The efficiency of the following cycles decreases quickly. The photocatalytic efficiency of sample MS presents the same tendency. However, its efficiency is always lower than that of sample ALD. As the photocatalytic perform-ance of nanomaterials is significantly influenced by dif-ferent parameters, including bandgap, morphology, surface area, particle size, crystallinity, and surface de-fect, in contrast to the structural and optical properties of the two samples, sample ALD owns a larger surface area and surface curvature effect, better crystallinity, and higher absorption, which leads to more active sites, eas-ier mass transportation, faster rate of reactions, and im-proved dye mineralization efficiency.
For comparison, the photodegradation of MB dye in Si nanowire arrays was also carried out. Figure 8 presents the absorption spectra of MB aqueous solutions as cata-lyzed by Si nanowire arrays under UV light. Besides a blue shift of the absorption peak, the spectral intensity of the MB solution is also reduced after photodegrada-tion in the catalyst, indicating the photocatalytic ability of the specimen. The photocatalytic efficiency is also cal-culated and shown in Table 1. The efficiency of the spe-cimen decreases in the same way as those hybrid nanowire arrays, but the decreasing rate is slower than the others. It reduces only ~5% in the 3 h, while the others reduce nearly twice as much. Moreover, the effi-ciency of the Si nanowire arrays in the first hour is in between those of sample ALD and sample MS. The effi-ciency difference may be primarily ascribed to the struc-tural characteristic of each sample. For sample MS, the branched ZnO nanowires mainly grow on the top of Si[image:6.595.57.290.543.712.2]
backbones. The long branches (1 μm) cross together, which blocks the transportation of MB dye from the top to the bottom, and only supplies the active sites on the top. However, for sample ALD, the branched ZnO nano-wires conformally grow on the whole sidewall of the Si nanowire. The length of the branches is only 500 nm, which leaves enough gap for the dye transportation. Therefore, in addition to the p–n junction that promotes the separation of photoinduced charge carriers and lowers electron-hole recombination, sample ALD pro-vides abundant surface states for the photodegradation, resulting in the highest efficiency.
It has been confirmed that the photodegradation of or-ganic dye pollutants in the semiconductor catalysts is due to the presence of active species, including hydroxyl radical ⋅OH, photogenerated hole h+, and superoxide anion radical⋅O−2 . According to the obtained results, the mechanisms underlying the photocatalytic activity of tree-like ZnO/Si nanowire arrays towards the degrad-ation of MB dye may be described as follows and be schematically illustrated in Fig. 9. The UV light induces electron-hole pair separation in the valence bands of ZnO and Si, and excites the electrons to their conduc-tion bands. As the conducconduc-tion and valence band edges of ZnO branches straddle those of p-type Si backbones , and the conduction band of ZnO is lower than that of Si, the free electrons in the conduction band of Si
prefer to flow to the conduction band of ZnO. Moreover, some part of electrons may also directly jump from the valence band of Si to the conduction band of ZnO in the interface of the heterojunction. The photogenerated electrons in the conduction bands of ZnO are captured by oxygen molecules that adsorbed on the ZnO surface to generate ⋅O−2 species, while the holes in the valence bands of Si react with water molecules or hydroxide anion in the solution to produce ⋅OH and h+ species, both of which cause the decomposition of organic dye molecules. The oxygen vacancies and carbon species in the nanotrees may also enhance the photocatalytic per-formance as they can serve as electron traps for the fast capture of photoexcited electrons, which forbids the re-combination of photogenerated electrons and holes. It’s conjectured that the⋅O−2 species in the system may play a dominant role in the degradation of MB dye, as the nanowires provide direct path for the electron transpor-tation and enough surface area in the tree branches to contact with the dye molecules. This can be detected by adding scavengers in the solution and will be studied in our further experiment.
As we can see in Fig. 7a, b, the photocatalytic efficiency of both the samples decreases with increasing irradiation period. There may be two reasons for the phenomena. One is the dissolution of ZnO/Si nanowires in the process of photocatalysis under UV light, the other is[image:7.595.56.522.214.171.124]
Fig. 7Absorption spectra of degraded MB aqueous solutions as catalyzed by sample ALD (a) and sample MS (b) under irradiation of UV light, in which 0, 1st, 2nd, and 3rd hours represent spectrum of MB solution before photodegradation, after photodegradation in the 1st, 2nd, and 3rd hours, respectively
Table 1Photodegradation efficiency of MB solution as catalyzed by sample ALD, sample MS and Si nanowire arrays in Figs. 7, 8, and 13
Time Sample ALD Sample MS Si nanowires Sample ALD in coating layer
1st hour 15.26% 9.93% 12.33% 11.52%
2nd hour 10.36% 7.75% 11.15% 11.47%[image:7.595.55.540.675.732.2]
the inactive surface as the illuminated area becomes less negatively charged during the photocatalytic process when the positive holes are drawn to illuminated area by the space charge layer . The function for the latter case can be recovered as a memory effect after a dark night interval. Figure 10 shows the cross-sectional SEM images of sample ALD and sample MS before and after photocatalysis. For sample ALD in Fig. 10a, b, the branched ZnO nanowires become sparse, short, and massive after photocatalysis. But for sample MS in Fig. 10c, d, the change is not so obvious. The ZnO branches seem to keep stable after the photocatalysis. Therefore, the dissolution of ZnO branches may play a critical role in the declining catalytic effect of sample ALD, whereas the inactive surface for the charge loss is a vital factor affecting the catalytic effect of sample MS. This difference is also corroborated by XPS spectra (see Additional file 1). The intensity under the deconvoluted peaks related to the Zn bond of sample ALD is reduced after the photocatalytic performance, while that of sam-ple MS is enhanced in the process. As the intensity responds to the amount of the binding bond, the
decreasing intensity indicates the loss of ZnO in sample ALD, whereas the enhancing intensity demonstrates the rise or stable state of ZnO in sample MS.
To solve this dissolution problem and improve the photocatalytic efficiency, sample ALD was coated by a layer of Ag nanoparticles by solution photoreduction and a TiO2film by ALD. The Ag nonoparticles on the
surface of the nanowire arrays induce a Schottky junc-tion between Ag and ZnO, which creates an internal electric field close to the interface and results in a de-crease of the recombination rate of the photogenerated electrons and holes . Moreover, the Ag nanoparticles exhibit localized surface plasmon resonance absorption of light which can significantly enhance semiconductor photocatalysis. On the other hand, TiO2has been widely
used as a protective layer for different semiconductor photoelectrodes due to its high resistance to corrosion and decomposition . Figure 11 shows the SEM images of the hybrid nanowires coated by TiO2, Ag, Ag/TiO2,
and TiO2/Ag, respectively. For comparison, the image of
the pristine trees is also supplied in it. The reduced Ag particles exhibit a ball-like structure with the diameter in a range of 100–360 nm, as estimated from the ampli-fied image of trees coated by Ag in Fig. 11f. The morph-ology of the samples in TiO2, Ag, and TiO2/Ag coating
layers seems to stay the same as that of the pristine trees, suggesting the conformal ability of the coating methods. However, for the sample with Ag/TiO2coating
layer in Fig. 11d, the branches seem a bit denser than the others, which may be due to the observation direc-tion with a smaller tilting angle. The coating layer of the sample is bigger than the others. They can be obviously seen with different structures. This is because the TiO2
layer is also deposited on the surface of the Ag particles. In this case, it provides a protective layer for the pristine trees as well as for the Ag particles. Figure 12 presents the reflection spectra of sample ALD with the coating layer. When the trees are coated by TiO2, the reflectance
peak originating from the bandgap absorption gets a red shift. This is because the bandgap of TiO2 is smaller
than that of ZnO. After the trees are coated by Ag parti-cles, a broad band at ~315 nm arises, and the intensity
Fig. 8Absorption spectra of degraded MB aqueous solutions as catalyzed by silicon nanowire arrays under irradiation of UV light, in which 0, 1st, 2nd, and 3rd hours represent spectrum of MB solution before photodegradation, after photodegradation in the 1st, 2nd, and 3rd hours, respectively[image:8.595.57.2126.96.36.199] [image:8.595.63.540.606.713.2]
of the characteristic peak of ZnO is reduced. The phenomenon can be ascribed to the presence of the reson-ance absorption of the Ag particles . When the trees are coated by both Ag and TiO2, the band and the peak
can be simultaneously observed, but their relative intensity is modulated by the relative position of the Ag and TiO2.
We had examined photocatalytic activity of the hybrid nanowires in these coating layers and found that only the sample coated with Ag/TiO2 exhibited a stable
photocatalytic performance. Figure 13 shows the absorp-tion spectra of degraded MB soluabsorp-tions as catalyzed by sample ALD in the coating layer. The specimen presents a good recycling ability. The intensity of the absorption
peak also increases for the latter degraded MB solution, but the change becomes very small. The acquired photo-catalytic efficiency, as shown in Table 1, only decreases 0.56% in the 3 cycles. Nevertheless, in contrast to the efficiency of sample ALD without coating layer in the first hour, the efficiency of the specimen decreases about 4%, which may be assigned to the low conductivity and kinetic limitation of TiO2, as well as the shielding effect
of the covered layer. The efficiency can be further improved by adjusting the diameter and length of both Si backbones and ZnO branches, the thickness of Ag layer and TiO2layer, or selecting other noble metal and[image:9.595.57.540.89.333.2]
Fig. 10Cross-sectional view SEM images of sample ALD (a,b) and sample MS (c,d) before and after photocatalytic performance[image:9.595.56.539.539.702.2]
ZnO/Si nanowire arrays with hierarchical structure were prepared by wet chemical etching and hydrothermal growth. The morphology, crystal structure, optical prop-erties, and photocatalysis efficiency of the system were significantly influenced by the ZnO seed layer. In con-trast to the seed layer deposited by MS, the more uni-form seed layer deposited by ALD resulted in ZnO branches with better crystallinity grown on the whole sidewall of the Si backbones, in addition to the stronger light absorption and higher photodegradation efficiency of MB for its larger surface area and higher surface curvature effect. The photocatalytic efficiency of the
system was declined under prolonging catalytic period, which might suffer from photodissolution and memory effect. A possible mechanism for the charge separation and organic dye pollutant degradation was proposed, and the stability and recycling ability of the system were improved by coating a layer of noble metal and metal oxide. All these suggested that the hybrid nanowires could find potential applications in photocatalysis and other fields, such as photovoltaics and sensors.
Additional file 1: Figure S1.High resolution XPS spectra of ZnO/Si nanowire arrays before and after photocatalysis. (a1–a3) Deconvolution of C (1s), O (1s), and Zn (2p) core levels in sample ALD before photocatalysis. (b1–b3) Deconvolution of C (1s), O (1s), and Zn (2p) core levels in sample ALD after photocatalysis. (c1–c3) Deconvolution of C (1s), O (1s), and Zn (2p) core levels in sample MS before photocatalysis. (d1–d3) Deconvolution of C (1s), O (1s), and Zn (2p) core levels in sample MS after photocatalysis.Figure S2. Spectral intensity of different bonds after photocatalysis (I) in contrast to that of before photocatalysis (I0) for sample ALD and sample MS as calculated from the deconvoluted spectra inFigure S1.(i) C-C bond, (ii) C-Zn bond, (iii) O-Zn bond, (iv) O-H bond or oxygen vacancies, (v) O-Zn 2p3/2, and (vi) Zn 2p1/2. (DOC 307 kb)
This work was supported by the National Key Research and Development Program of China (2016YFB0400801), 863 program (2014AA032608), National Natural Science Foundation of China (U1405253, 61227009, 61205051, 90921002), Natural Science Foundation of Fujian Province of China (2016 J01265, 2013 J05097), Fundamental Research Funds for the Central Universities (20720160015, 20720150032), and Fundamental Research Funds for Xiamen University (2016Y0589, 2016Y0591).
Availability of Data and Materials
Supporting information contains XPS spectra of sample ALD and sample MS before and after photocatalysis as well as their relative intensity of the deconvoluted peaks.
DL, XY, and CL performed the experiments, analyzed the data, and drafted the manuscript. SH designed the experiment, analyzed the data, and revised the manuscript. BH, QY, BY, and XH helped prepare and characterize the samples and analyze the data. ZRT, JL, JW, HZ, SL, and JK participated in the final data analysis and critical review of the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
1Fujian Provincial Key Laboratory of Semiconductors and Applications,
Collaborative Innovation Center for Optoelectronic Semiconductors and Efficient Devices, Department of Physics, Xiamen University, Xiamen 361005, China.2Department of Chemistry and Biochemistry, University of Arkansas, Fayetteville, AR 72701, USA.3State Key Lab of Silicon Materials, Zhejiang University, Hangzhou 310027, China.4Fujian Provincial Key Laboratory of Eco-Industrial Green Technology, Wuyi University, Fujian 354300, China.
Received: 29 September 2016 Accepted: 18 December 2016
1. Wang R, Guo J, Chen D, Miao Y, Pan J, Tjiub W, Liu T (2011)“Tube brush” like ZnO/SiO2hybrid to construct a flexible membrane with enhanced photocatalytic properties and recycling ability. J Mater Chem 21:19375–19380
Fig. 12Diffuse reflection spectra of sample ALD with the coating layer. The spectra of trees in other coating layers were shifted upward in contrast to the spectrum of trees coated by TiO2 for comparison[image:10.595.56.291.499.663.2]
2. Kargar A, Sun K, Kim S, Lu D, Jing Y, Liu Z, Pan X, Wang D (2013) Three-dimensional ZnO/Si broom-like nanowire heterostructures as
photoelectrochemical anodes for solar energy conversion. Phys Status Solidi A 210:2561–2568
3. Tong H, Ouyang S, Bi Y, Umezawa N, Oshikiri M, Ye J (2012) Nano-photocatalytic materials: possibilities and challenges. Adv Mater 24:229–251 4. Cheng C, Fan H (2012) Branched nanowires: synthesis and energy
applications. Nano Today 7:327–343
5. Bierman M, Jin S (2009) Potential applications of hierarchical branching nanowires in solar energy conversion. Energy Environ Sci 2:1050–1059 6. Doerk G, Ferralis N, Carraro C, Maboudian R (2008) Growth of branching Si
nanowires seeded by Au–Si surface migration. J Mater Chem 18:5376–5381 7. Boettcher S, Spurgeon J, Putnam M, Warren E, Turner-Evans D, Kelzenberg M, Maiolo J, Atwater H, Lewis N (2010) Energy-conversion properties of vapor-liquid-solid–grown silicon wire-array photocathodes. Science 327:185–187 8. Chen Y, Prange J, Duhnen S, Park Y, Gunji M, Chidsey C, McIntyre P (2011)
Atomic layer-deposited tunnel oxide stabilizes silicon photoanodes for water oxidation. Nat Mater 10:539–544
9. Li C, Usami K, Mizuta H, Oda S (2011) Growth of Ge–Si nanowire
heterostructures via chemical vapor deposition. Thin Solid Films 519:4174–4176 10. Dick K, Deppert K, Larsson M, Martensson T, Seifert W, Wallenberg L,
Samuelson L (2004) Synthesis of branched‘nanotrees’by controlled seeding of multiple branching events. Nat Mater 3:380–384
11. Wang D, Qian F, Yang C, Zhong Z, Lieber C (2004) Rational growth of branched and hyperbranched nanowire structures. Nano Lett 4:871–874 12. Dick K, Deppert K, Karlsson L, Seifert W, Wallenberg L, Samuelson L (2006)
Position-controlled interconnected InAs nanowire networks. Nano Lett 6: 2842–2847
13. Bierman M, Lau Y, Kvit A, Schmitt A, Jin S (2008) Dislocation-driven nanowire growth and Eshelby twist. Science 320:1060–1063
14. Hull K, Grebinski J, Kosel T, Kuno M (2008) Induced branching in confined PbSe nanowires. Chem Mater 17:4416–4425
15. Manna L, Milliron D, Meisel A, Scher E, Alivisatos A (2003) Controlled growth of tetrapod-branched inorganic nanocrystals. Nat Mater 2:382–385 16. Jung Y, Ko D, Agarwal R (2007) Synthesis and structural characterization of
single-crystalline branched nanowire heterostructures. Nano Lett 7:264–268 17. Baek S, Kim S, Shin J, Kim J (2012) Preparation of hybrid silicon wire and
planar solar cells having ZnO antireflection coating by all-solution processes. Sol Energy Mater Sol Cells 96:251–256
18. Sun K, Jing Y, Li C, Zhang X, Aguinaldo R, Kargar A, Madsen K, Banu K, Zhou Y, Bando Y, Liu Z, Wang D (2012) 3D branched nanowire heterojunction photoelectrodes for high-efficiency solar water splitting and H2generation. Nanoscale 4:1515–1521
19. Sun K, Jing Y, Park N, Li C, Bando Y, Wang D (2010) Solution synthesis of large-scale, high-sensitivity ZnO/Si hierarchical nanoheterostructure photodetectors. J Am Chem Soc 132:15465–15467
20. Kargar A, Sun K, Jing Y, Choi C, Jeong H, Zhou Y, Madsen K, Naughton P, Jin S, Jung G, Wang D (2013) Tailoring n-ZnO/p-Si branched nanowire heterostructures for selective photoelectrochemical water oxidation or reduction. Nano Lett 13:3017–3022
21. Sheng W, Sun B, Shi T, Tan X, Peng Z, Liao G (2014) Quantum dot-sensitized hierarchical micro/nanowire architecture for photoelectrochemical water splitting. ACS Nano 8:7163–7169
22. Cheng P, Liu Y, Sun P, Du S, Cai Y, Liu F, Zheng J, Lu G (2014)
Hydrothermally growth of novel hierarchical structures titanium dioxide for high efficiency dye-sensitized solar cells. J Power Sources 268:19–24 23. Lao J, Wen J, Ren Z (2002) Hierarchical ZnO nanostructures. Nano Lett 2:
24. Cesar I, Sivula K, Kay A, Zboril R, Graetzel M (2009) Influence of feature size, film thickness, and silicon doping on the performance of nanostructured hematite photoanodes for solar water splitting. J Phys Chem C 113:772–782 25. McCune M, Zhang W, Deng Y (2012) High efficiency dye-sensitized solar
cells based on three-dimensional multilayered ZnO nanowire arrays with
“caterpillar-like”structure. Nano Lett 12:3656–3662
26. Cheng C, Yan B, Wong S, Li X, Zhou W, Yu T, Shen Z, Yu H, Fan H (2010) Fabrication and SERS performance of silver-nanoparticle-decorated Si/ZnO nanotrees in ordered arrays. ACS Appl Mater Interfaces 2:1824–1828 27. Song H, Zhang W, Cheng C, Tang B, Luo L, Chen X, Luan C, Meng X, Zapien J,
Wang N, Lee C, Bello I, Lee S (2011) Controllable fabrication of three-dimensional radial ZnO nanowire/silicon microrod hybrid architectures. Cryst Growth Des 11: 147–153
28. Kuriakose S, Choudhary V, Satpati B, Mohapatra S (2014) Enhanced photocatalytic activity of Ag–ZnO hybrid plasmonic nanostructures prepared by a facile wet chemical method. Beilstein J Nanotechnol 5:639– 650
29. Chang S, Chuang V, Boles S, Thompson C (2010) Metal-catalyzed etching of vertically aligned polysilicon and amorphous silicon nanowire arrays by etching direction confinement. Adv Funct Mater 20:4364–4370
30. Han J, Qiu W, Gao W (2010) Potential Dissolution and photo-dissolution of ZnO thin films. J Hazard Mater 178:115–122
31. Meng X, Lin B, Fu Z (2007) Influence of CH3COO−on the room temperature photoluminescence of ZnO films prepared by CVD. J Lumin 126:203–206 32. Samadi M, Shivaee H, Pourjavadi A, Moshfegh A (2013) Synergism of
oxygen vacancy and carbonaceous species on enhanced photocatalytic activity of electrospun ZnO-carbon nanofibers: charge carrier scavengers mechanism. Appl Catal A-Gen 466:153–160
33. Zeng H, Duan G, Li Y, Yang S, Xu X, Cai W (2010) Blue Luminescence of ZnO nanoparticles based on non-equilibrium processes: defect origins and emission controls. Adv Funct Mater 20:561–572
34. Tay Y, Tan T, Boey F, Liang M, Ye J, Zhao Y, Norby T, Li S (2010) Correlation between the characteristic green emissions and specific defects of ZnO. Phys Chem Chem Phys 12:2373–2379
35. Huang N, Shu J, Wang Z, Chen M, Ren C, Zhang W (2015) One-step pyrolytic synthesis of ZnO nanorods with enhanced photocatalytic activity and high photostability under visible light and UV light irradiation. J Alloys Compd 648:919–929
36. Huang S, Yang Q, Yu B, Li D, Zhao R, Li S, Kang J (2014) Controllable synthesis of branched ZnO/Si nanowire arrays with hierarchical structure. Nanoscale Res Lett 9:328, 1-9
37. Yassitepe E, Yatmaz H, Ozturk C, Ozturk K, Duran C (2008) Photocatalytic efficiency of ZnO plates in degradation of azo dye solutions. J Photochem Photobiol A 198:1–6
Submit your manuscript to a
journal and beneﬁ t from:
7Convenient online submission
7Rigorous peer review
7Immediate publication on acceptance
7Open access: articles freely available online
7High visibility within the ﬁ eld
7Retaining the copyright to your article